at SciVerse ScienceDirect
International Biodeterioration & Biodegradation 83 (2013) 97e104Contents lists availableInternational Biodeterioration & Biodegradation
journal homepage: www.elsevier .com/locate/ ibiodAntifouling paints based on marine natural products from ColombianCaribbean
Marisol Santos Acevedo a,1, Carlos Puentes a,1, Katerine Carreo a,1, Javier Gmez Len a,1,Mirta Stupak b,2, Mnica Garca b,2, Miriam Prez b,c,2, Guillermo Blustein b,d,*a Instituto de Investigaciones Marinas y Costeras e INVEMAR, Cerro Punta de Betn, Santa Marta, ColombiabCentro de Investigacin y Desarrollo en Tecnologa de Pinturas e CIDEPINT, 52 e/121 y 122, La Plata, ArgentinacUniversidad Nacional de La Plata e Facultad de Ciencias Naturales y Museo, ArgentinadUniversidad Nacional de La Plata e Facultad de Ciencias Agrarias y Forestales, Argentinaa r t i c l e i n f o
Article history:Received 26 December 2012Received in revised form30 April 2013Accepted 3 May 2013Available online 1 June 2013
Keywords:BiofoulingSpongesSea cucumberAntifouling paints* Corresponding author. Centro de Investigacin yPinturas e CIDEPINT, 52 e/121 y 122, La Plata, Argentin
E-mail address: email@example.com (G. Blu1 Tel.: 57 5 4328600x231.2 Tel.: 54 221 483 1141/44.
0964-8305/$ e see front matter 2013 Elsevier Ltd.http://dx.doi.org/10.1016/j.ibiod.2013.05.002a b s t r a c t
Biofouling control involves the application of paints containing toxic substances to the marineecosystem. One of the most promising alternative technologies to antifouling paints based on heavymetals is the development of coatings whose active ingredients are compounds naturally occurring inmarine organisms. This study investigated the antifouling activity of organic extracts from someepibiont-free Colombian Caribbean Sea sponges (Agelas tabulata, Myrmekioderma gyroderma, Oceanapiapeltata, Aplysina lacunosa, Neopetrosia sp.) and a sea-cucumber (Holoturia glaberrima). Extracts wereincorporated into hard stable gels and into soluble matrix antifouling paints and exposed in the sea(Colombia and Argentina). After 45 and 90 days, significant differences in fouling cover percentagesbetween painted panels and controls were found (p < 0.05). It was demonstrated that the greatestantifouling activity was contained in extracts of A. tabulata and Holoturia glaberrima in both study sites.This study successfully identified potential new sources of natural antifouling compounds.
2013 Elsevier Ltd. All rights reserved.1. Introduction
Marine biofouling is an extensive phenomenon causing largeproblems to engineered structures such as ships and offshoreplatforms by way of increased use of manpower, fuel, material anddry-docking time. Shipping accounts for approximately 90% ofworld trade and seaborne trade has quadrupled over the past threedecades (ICS and ISF, 2009). The economic costs of hull fouling havebeen a driving force behind the development of antifouling tech-nologies, a global industry that is now worth approximately US$ 4billion annually (Wright, 2009).
Antifouling paints have traditionally incorporated toxicantsincluding copper and tributyltin into a matrix that graduallyleaches the biocide from the surface layer to prevent settlement.However, these compounds, particularly TBT, were reported to behighly toxic and persistent in the marine environment, and provedDesarrollo en Tecnologa dea. Tel.: 54 221 483 1141/44.stein).
All rights reserved.to have adverse effects on non-target organisms (Alzieu et al., 1989;Claisse and Alzieu, 1993; Yebra et al., 2004; Limna Mol et al., 2009;Prez et al., 2009). Because of its toxicity, a worldwide ban on TBTwent into effect in 2008.
Increased awareness of the impacts resulting from the use oftoxic antifouling paints has prompted investment in the researchand development of non-toxic alternatives such as coatings thatincorporate natural origin compounds as derivates from algae andother marine organisms (Holmstrom and Kjelleberg, 1994;Kjelleberg and Steinberg, 1994; De Nys et al., 1995; Rittschof, 2000;Hellio et al., 2002, 2009).
In the marine environment, where all surfaces are constantlyexposed to colonization, many sessile organisms remain relativelyfree of biofouling. Marine invertebrates are a potential source ofnatural, bioactive products that act against external threats(Sipkema et al., 2005; Paul et al., 2006). They are involved in a greatvariety of interactions, many of which are chemically mediated(Paul et al., 2006; Egan et al., 2008). These compounds often playmultiple ecological roles, primarily protection against predators(Pawlik et al., 1995; Waddell and Pawlik, 2000; Burns et al., 2003;Ruzicka and Gleason, 2009), competitors for space (Engel andPawlik, 2000; Luter and Duckworth, 2010), biofoulers (Becerroet al., 1994) and opportunistic pathogenic microorganisms
Delta:1_given nameDelta:1_surnameDelta:1_given nameDelta:1_surnameDelta:1_given nameDelta:1_surnameDelta:1_given nameDelta:1_surnamemailto:firstname.lastname@example.org://crossmark.dyndns.org/dialog/?doi=10.1016/j.ibiod.2013.05.002&domain=pdfwww.sciencedirect.com/science/journal/09648305http://www.elsevier.com/locate/ibiodhttp://dx.doi.org/10.1016/j.ibiod.2013.05.002http://dx.doi.org/10.1016/j.ibiod.2013.05.002http://dx.doi.org/10.1016/j.ibiod.2013.05.002
Fig. 1. Species studied. (a) Agelas tubulata, (b) Aplysina lacunosa, (c) Biemna cribaria, (d) Myrmekioderma gyroderma, (e) Oceanapia peltata, (f) Neopetrosia proxima, (g) Spirastrellacoccnea, (h) Holothuria glaberrima.
M.S. Acevedo et al. / International Biodeterioration & Biodegradation 83 (2013) 97e10498(Newbold et al., 1999; Kelman et al., 2001). Particularly, secondarymetabolites produced by marine sessile organisms represent a newperspective on preventing overgrowth by epibionts and couldpotentially be used as commercial antifoulants (Willemsen andFerrari, 1993).
Sponges, with their rich chemical defense mechanisms, areamong the most studied organisms for the isolation of naturalproducts antifoulants (NPAs) (Thakur and Anil, 2000). Marinesponges have received much attention because they represent asource of unique and diverse secondary metabolites with novelstructures and potential biological activities (Becerro et al., 1997;Thacker et al., 1998; Sera et al., 1999; Schupp et al., 1999; Faulkner,2000, 2002; Matsunaga et al., 2000; Harper et al., 2001; Blunt et al.,2003; Dobretsov et al., 2005; Stowe et al., 2011). Previous studieshave shown that sponges are rich in terpenoids and steroids whichcan function in antipredation, competition for space and control ofepibionts (Becerro et al., 2003; Hellio et al., 2005; Clavico et al.,2006; Tsoukatou et al., 2007).
In contrast, echinoderms are one of the groups less explored inrelation with NPAs. Only a few investigations of antifouling com-pounds have been examined with starfish, basket stars and seaurchins (Bryan et al., 1996; DeMarino et al., 1997; Haug et al., 2002).
M.S. Acevedo et al. / International Biodeterioration & Biodegradation 83 (2013) 97e104 99However, sea cucumbers are a large and diverse group of organismsfrom which a wide range of secondary metabolites have been iso-lated. A number of these compounds possess biological activitysuch as toxicity, antibacterial, antifungal, antiviral, anti-tumor andother specific activities (Bryan et al., 1992; Villasin and Pomory,2000; Haug et al., 2002; Han et al., 2009).
The properties established for both, sponges and sea cucumbers,and particularly their antimicrobial activity, support the hypothesisthat these groups could be potential candidates to obtain anti-fouling compounds. The inhibition of the organism settlementprocess could be achieved by breaking one or more of the stepsimplicated in biofouling development (Hellio et al., 2001). Addi-tionally, bacterial biofilms can play an important role in mediatingsettlement and metamorphosis of larvae, e.g. they can enhance orinhibit larval and algal spore attachment.
Most of the experiments conducted to evaluate antifouling ac-tivity of a vast range of substances have been laboratory-based usingdifferent larval stages, and also field tests employing gels containingextracts (Henrikson and Pawlik, 1995, 1998). However, few of thesesubstances have incorporated into marine paints for testing.
In this paper, the antifouling properties of seven sponge extractsAgelas tubulata (Schmidt, 1870), Aplysina lacunosa (Lamarck, 1814),Biemna cribaria (Alcolado and Gotera, 1986), Myrmekiodermagyroderma (Alcolado, 1984), Neopetrosia proxima (Duchassaing andMichelotti, 1864), Oceanapia peltata (Schmidt, 1870) and Spirastrellacoccinea, and a sea cucumber, Holothuria glaberrima (Selenka,1867), from the Caribbean Colombian Sea included into an inert gel(Phytagel) and into a paint matrix were examined. Effectivenessof extracts was evaluated in two different harbous, Santa Marta(Colombia) and Mar del Plata (Argentina).
2. Material and methods
2.1. Extraction procedure
Extracts were obtained from hand-collected marine organismsby Scuba diving in the Colombian coast from Santa Marta toNeguanje (Tayrona National Park, 111905200Ne740502800W). Sevenmarine sponge species (A. tubulata, Aplysina lacunosa, Biemna cri-baria, Mymekioderma gyroderma, Neopetrosia proxima, Oceanapiapeltata and Spirastrella coccinea), and a sea cucumber (H. glaberrima)were selected for the experiments (Fig. 1).
Organism surfaces were free of macroepibionts and had no evi-dence of depredation. For the experiments, tissues were rinsed toremove debris and cut in small pieces, and wet weights were deter-mined. Sponges and holothurians were stored at 15 C until pro-cessed. Then, sampleswere lyophilized (36e48h/45 C/0.120mbar)in order to eliminate water from tissues and dry weights recorded.
Dry tissues were macerated